Sintering Effect on the Microstructure and Mechanical ... SINTERING EFFECT ON THE MICROSTRUCTURE AND...
Embed Size (px)
Transcript of Sintering Effect on the Microstructure and Mechanical ... SINTERING EFFECT ON THE MICROSTRUCTURE AND...
SINTERING EFFECT ON THE MICROSTRUCTURE AND MECHANICAL
PROPERTIES OF ALLOY 718 PROCESSED BY POWDER INJECTION MOLDING
J. J. Valencia*, J. Spirko*9 and R. Schmees**
*Concurrent Technologies Corporation, 1450 Scalp Avenue, Johnstown, PA 15904 **United Technologies, Pratt & Whitney, West Palm Beach, FL 33410
Powder injection molding (PIM) is an emerging technology for manufacturing gas turbine engine components. To evaluate superalloy alloy 718 for these applications, mechanical testing specimens were produced by PIM and sintered at various heating rates in a partial pressure of argon. Alloy 718 is difficult to process because a low melting point eutectic-Laves phase develops during the sintering process. The Laves phase prevents full densilication and decreases the tensile properties. Heating ramp rates up to lSC/min and a holding time of 6 hours prevented the formation of Laves phase during sintering. In the as-sintered condition, 99% of the theoretical density was achieved. After HIP and heat treatment, the tensile properties at room temperature and 650C exceeded the minimum property requirements, while stress rupture time, high cycle fatigue, and creep properties met typical aerospace properties. Stress rupture elongation life was met with an additional delta heat treatment.
This work was conducted by the National Center for Excellence in Metalworking Technology, operated by Concurrent Technologies Corporation under contract No. N00140-92-C-BC49 to the U.S. Navy as part of the U.S. Navy Manufacturing and Technology Program
Superalloys 718, 625, 706 and Various Derivatives Edited by E.A. Loria
The Minerals, Metals &Materials Society, 1997
Wrought components made from alloy 718 have gained considerable acceptance in the manufacturing of high-performance turbine engine components. Many of these components are highly complex shapes which are very expensive to produce due to extensive machining. Casting does not yield material suitable for these applications because of segregation and microstructural inhomogeneity. The same is true of press and sinter P/M processes because of the shape complexity and dimensional tolerances which cannot be achieved without extensive machining operations.
Powder injection molding (PIM) is an emerging technology for the cost-effective production of large numbers of small metal parts. PIM also has the ability to manufacture components with complex geometry and very close dimensional tolerances. In spite of the obvious cost advantage, PIM has not been implemented for the production of alloy 718 turbine engine components. The reasons for this are because of the stringent mechanical property requirements for aerospace components, and the very limited engineering knowledge database of PIM alloy 718 [l-3].
The objective of this work is to optimize the thermal consolidation of PIM alloy 718 to achieve the mechanical property requirements of aerospace material specification AMS 5596 . To do this, the effect of sintering parameters on the microstructure and mechanical properties are examined.
A PIM feedstock was prepared from gas-atomized alloy 718 powder with a mean particle size of 15 nm and a proprietary polymer-based binder to approximately 64% solids loading . Tensile, stress rupture, creep, and high-cycle fatigue specimens were injection-molded to dimensionally comply with the ASTM standards. The specimens were solvent debound followed by thermal debinding and pre-sintering at 1090C for 2 hours in a hydrogen atmosphere.
Sintering was conducted at 1260C for 6 hours in vacuum with an argon partial pressure of approximately 1000 microns of mercury to prevent chromium evaporation of the alloy. To achieve the maximum sintering temperature, three heating ramp rates from room temperature were used including (1) lC/min, (2) lOC/min, and (3) 15CYmin. The sintered specimens were hot isostatically pressed (HIP) at 1190C for 4 hours at 103.5 MPa (15 Ksi).
Heat treatment was conducted per AMS 5663 specification . Solution treatment was performed at 950C for 1 hour in argon followed by air cooling. Precipitation treatment was conducted at 718C for 8 hours, followed by furnace cooling at 38C per hour to 620C holding for 8 hours, and then air cooling. Prior to the solution heat treatment, the stress rupture specimens were heat-treated at 870C for 10 hours to increase the amount of the orthorhombic Do, structure, or equilibrium Ni,Nb Z-phase at the grain boundaries.
The specimen density was measured by the Archimedes method. Tensile properties were measured at room temperature and at 650C. Stress rupture, high-cycle fatigue (HCF), and creep were also measured at 650C. Microstructural analyses were conducted on selected samples using optical metallography and scanning electron microscopy (SEM) coupled with energy dispersion spectroscopy (EDS). Fracture analysis was performed by SEM.
Results and Discussion
Sintering Effects on Density and Microstructure
Table I compares the effect of the sintering rate on the density of the PIM alloy 718 sintered at 1260C for 6 hours. The table also shows the heat treatment (HT) effect on the density for the various materials. The HIP effect on density is only shown for the alloy heated at a ramp rate of 15CYmin. The density of the heat-treated wrought alloy 718 is also provided for comparison.
The lowest as-sintered density was observed at a heating rate of lOC/min, and the highest was obtained at lSC/min. HT+HIP increased the sintered density at all ramp rates. However, the density of wrought alloy 718 is still higher than any of the PIM specimens.
Table I - Effect of Sintering Heating Rate on Density of PIM Alloy 718 Sintered at 1260C for 6 Hours.
Early studies showed that density increases with an increase in the heating ramp rate during the sintering process . In the present work, this observation is confirmed from lOC/min to lSC/min. However, the heating ramp rate of lOC/min yielded the lowest sinter density. One explanation for this observation is the formation of heavy intermetallic Nb-bearing yllaves eutectic phase at -1170C [2, 6-81 which remains liquid at the sintering temperature. Also, the high content of heavy elements such as niobium and chromium in the Laves phase slows its dissolution into the matrix. At lC/min ramp rate, the Laves phase was formed; however, there was sufficient time to dissolve a relatively large amount of this phase into the matrix. While at lSC/min, the Laves phase does not have sufficient time to nucleate and grow in a significant nronortion. Therefore, it is reasonable to assume that undissolved liquid eutectic Laves phase (particularly at a heating rate of lOC/min) causes porosity during cooling. Figure 1 shows microstructures for the various sintering rates.
Figure 1 - SEM views of PIM alloy 718 in the as-sintered condition: (a) lC/min. (b) lOC/min. (c) lYC/min.
Note that the porosity is associated with the eutectic Laves phase primarily at lOC/min. (Figure lb). The eutectic Laves at lOC/min. and lSC/min. heating rates were found in a very small proportion (< 0.5 percent).
Table II shows the effect of the heating rate on the PIM 718 microstructure including total fraction of second phases (primarily identified as Laves and 6 phases), average grain size, and grain-size range. Note that the proportion of Laves and 6 phases was higher at lOC/min and lower at lSC/min. HIP+HT increased the amount of the second phases; however, at 1 C/min there is practically no change. A non-uniform grain size was observed in all as-sintered materials. However, the average grain size decreased with an increase in the sintering rate. HIP+HT had a minor effect on the grain size. These microstructural characteristics are shown in Figure 2.
Figure 2 - Light optical views of PIM alloy 718 in the HT and HIP+HT conditions: (a) and (b) 1Wmin.; (c) and (d) 1OWmin.; (e) and (f) 15Wmin. (HT: left, HIP and HT: right)
Table II - Microstructural Characteristics of PIM Alloy 718
The HIP+HT produced a more uniform distribution of the second phases at all sintering rates. EDS analyses shows that a large proportion of the second phases in the HIP+HT materials is the 6 phase. This is expected since some of the Laves phase was dissolved during holding at the HIP temperature (1190C for 4 hours). Then the 6 phase was formed during the slow cooling of the HIP furnace from above the 6 solvus (-1020C) . The 6 phase had two morphologies which included a plate-like morphology that was found at the grain boundaries, and a globular morphology which was found intragranularly. The Laves phase persisted after HIP and heat treatment. However, the larger proportion of this phase was found in specimens sintered at a heating ramp rate of lOC/min.
From all the PIM materials, the specimens sintered at a heating ramp rate of lOC/min showed a more uniform grain size (Figures 2c and 2d). This may be due to the larger proportion of Laves and F phases (primarily Laves in this case) produced during the sintering process. As shown in Figure 3, a small grain size is associated with the presence of Laves phases, which are present at the grain boundaries; this. suggests that Laves phases control the grain growth during sintering.
Figure 3 - SEM view of a PIM alloy 718 sintered at a heating rate of 15Wmin showing Laves phase at the grain boundaries.
The effects of surface grinding on the testing specimens, as well as the effect of testing temperature on the mechanical properties, have been discussed in a previous paper . The mechanical testing results pr